0 downloads
0 Views
466KB Size

Letter pubs.acs.org/JPCL

Predicting Band Gaps with Hybrid Density Functionals Alejandro J. Garza†,¶ and Gustavo E. Scuseria*,†,‡ †

Department of Chemistry and ‡Department of Physics and Astronomy, Rice University, Houston, Texas 77251-1892, United States S Supporting Information *

ABSTRACT: We compare the ability of four popular hybrid density functionals (B3LYP, B3PW91, HSE, and PBE0) for predicting band gaps of semiconductors and insulators over a large benchmark set using a consistent methodology. We observe no signiﬁcant statistical diﬀerence in their overall performance, although the screened hybrid HSE is more accurate for typical semiconductors. HSE can improve its accuracy for large band gap materialswithout aﬀecting that of semiconductorsby including a larger portion of Hartree−Fock exchange in its short-range. Given that screened hybrids are computationally much less expensive than their global counterparts, we conclude that they are a better option for the black box prediction of band gaps.

B

The present study focuses on band gap prediction by both short-range screened and global hybrids. We benchmark popular hybrids like HSE06 (henceforth referred to as simply HSE), B3PW91, B3LYP, and PBE0 (also known as PBEh or PBE1PBE). For this comparison, we utilize a variety of error measures in order to avoid the diﬃculties and ambiguities that emerge when trying to decide which electronic structure method is best for a determined task.10,11 We ﬁnd that these four functionals are similarly adequate for the calculation of band gaps; diﬀerent error measures for HSE, B3PW91, and B3LYP are very close to each other, and while PBE0 tends to overestimate band gaps, the error is systematic and straightforward to correct with a linear ﬁt. If the benchmark set is narrowed to traditional semiconductors, then HSE emerges as the winner. In addition, we show that short-range hybrids can describe even large band gap insulators by including an increased portion of HF exchange in the shortrange only. Due to their lower cost as compared to global hybrids, greater ease to achieve convergence, and overall good performance, we conclude that screened hybrids are a better option for the prediction of band gaps. Statistical Evaluation. We have carried out band gap calculations for 41 semiconductors and insulators using the GAUSSIAN13 suite of programs. The set includes materials from the SC40 data set,7 as well as transition metal oxides (FeO, CoO, NiO, MnO, and VO2) and large band gap salts (NaCl, LiCl, and LiF); the set is similar to that of ref 9 (some compounds have been excluded because spin−orbit eﬀects are very large and we have not used spin−orbit corrections in our calculations). As in that reference, we employed experimental geometries. The basis sets used for SC40 compounds are the same as those of ref 7 (which are similar or identical to those in

and structure calculations are an important application of electronic structure methods in materials science. Due to the cost of computing electronic properties for extended solids, density functional theory (DFT) methods are most often used for such calculations. However, local and semilocal density functional approximationsthe most aﬀordable type of Kohn− Sham functionals for solidsbadly underestimate the band gaps of semiconductors (the materials of principal interest in practical applications) and insulators due to self-interaction error.1,2 Hybrid functionals that incorporate a fraction of nonlocal Hartree−Fock (HF) exchange overcome this issue; however, computing HF exchange in solids is considerably more expensive than evaluating a semilocal density functional. Methods based on the GW approximation can also be used to compute band gaps more accurately, but these techniques are even more expensive than hybrids. A good compromise between cost and accuracy is provided by short-range screened hybrids, functionals that include HF exchange only for the short-range part of the electron−electron interaction, which signiﬁcantly reduces the cost of evaluating the nonlocal HF part of the exchange as compared to standard hybrids.3 These types of functionals have been shown to provide reasonably accurate band gaps for semiconductors, and variants of the Heyd− Scuseria−Ernzerhof3−7 (HSE) short-range hybrid have been widely used for the calculation of semiconductor band gaps for many years.8 A recent study9 declares the (standard) hybrid B3PW91 as the winner for resolving the band gap prediction problem for materials design. However, that study did not evaluate the performance of other hybrid functionals using a direct comparison based on a consistent methodology. We here carry out such detailed comparison. We also comment upon the pitfalls that arise when benchmarking density functionals,10,11 as well as aspects of computational eﬃciency for solids between short-range hybrids like HSE12 and standard global hybrids (by global, we mean standard full-range hybrids like B3PW91). © XXXX American Chemical Society

Received: August 10, 2016 Accepted: October 5, 2016

4165

DOI: 10.1021/acs.jpclett.6b01807 J. Phys. Chem. Lett. 2016, 7, 4165−4170

Letter

The Journal of Physical Chemistry Letters

nonlocal exchange, while HSE includes 25% but only in the short-range. Inclusion of larger fractions of exact exchange increases the calculated band gaps: PBE0 includes 25% fullrange HF exchange, which leads to an overestimation of the band gaps as compared to experiment and the other functionals; however, all four functionals underestimate very large insulator band gaps and follow the linear trend mentioned above. In fact, if one ﬁts the data in Figure 1 to a linear function, the slopes for the four hybrids diﬀer by no more than about 3% (see Table 1). HSE, however, has a linear ﬁt intercept much smaller than that of the global hybrids (0.36 eV as compared to 0.65, 0.63, and 0.95 eV for B3PW91, B3LYP, and PBE0, respectively), indicating better agreement with the experimental data. We now discuss the diﬀerent error measures in Table 1. The ﬁrst two, the mean error (ME) and the mean absolute error (MAE), are some of the most widely used error measures in quantum chemistry. The ME shows that HSE has a tendency to underestimate band gaps (−0.24 eV), while B3PW91 and B3LYP slightly overestimate (0.14 and 0.13 eV, respectively), and PBE0 signiﬁcantly overestimates (0.43 eV). On the basis of MAE, HSE predicts band gaps closer to experiment (MAE = 0.37 eV) and is closely followed by B3PW91 and B3LYP (0.44 eV for both). PBE0 has the worst MAE (0.59 eV) mainly due to the aforementioned tendency to overestimate band gaps. In terms of the mean absolute percent error (MAPE), HSE also comes out better (16%) than the other hybrids (27, 23, and 45% for B3PW91, B3LYP, and PBE0, respectively). The lower MAPE of HSE as compared to that of the other hybrids is more notable than its lower MAE, in part because the average error for HSE is increased substantially by the errors for the high band gap compounds; if the very large band gap (i.e., more than ∼8 eV) compounds are excluded, the MAEs for HSE, B3PW91, B3LYP, and PBE0 are 0.26, 0.37, 0.36, and 0.57 eV, respectively. Furthermore, if we consider only typical semiconductors for which low-temperature experimental band gaps are available (group 1 of the SC40 set; see ref 7), the MAEs (in the same order) are 0.18, 0.32, 0.31, and 0.55 eV, and the MAPEs are 17, 33, 26, and 62. We also report in Table 1 the standard deviations (SDs) of the error; a perfect approximation would have zero ME and zero SD. However, no signiﬁcant diﬀerence is observed between the SDs of the hybrids; the largest diﬀerence is 0.05 eV between HSE and PBE0. Note also that the functional with the worst ME and MAE, PBE0, has the smallest SD. Thus, as has been pointed out by Savin et al.,10,11 using diﬀerent error measures to judge the quality of a functional can lead to contradictory results.

ref 9), and the basis sets of ref 9 are used for the rest of the compounds. However, while we had no problems computing band gaps for all of these compounds with HSE, some of the global hybrid calculations (particularly PBE0) were too expensive or too diﬃcult to converge, even when starting from a converged HSE guess. Inaccuracies in building an approximate Fock matrix for full-range hybrids make these calculations harder to converge, especially for compounds with smaller gaps.14 We were thus unable to obtain results for all 41 compounds with global hybrids. The calculated vs experimental band gaps for the 27 compounds for which all four functionals successfully converged are shown in Figure 1 (see detailed data

Figure 1. Calculated vs experimental band gaps for the functionals studied here.

in the Supporting Information). Various statistics of the error (which we shall discuss in short and are a compilation of those presented in ref 10) for these calculations and for all of the compounds for which each functional converged are summarized in Table 1. As shown by the insigniﬁcant changes (∼0.01−0.03 eV) in the diﬀerent error measures when increasing the size of the benchmark set (from 27 to 41 for HSE, 37 for B3PW91, and 34 for B3LYP), the 27 compounds for which all four functionals converged are representative enough to get accurate estimates of the expected deviations from experiment for each functional. The ﬁrst thing that is noticeable from Figure 1 is that the four functionals follow the same, fairly linear, trend. Results from HSE, B3LYP, and B3PW91 are close together; the latter two in particular give extremely similar band gaps. This is most likely due to the incorporation of similar amounts of HF exchange; B3LYP and B3PW91 both have 20% full-range

Table 1. Diﬀerent Band Gap Prediction Error Measures for the Four Functionals Studied Here expt. size of test set mean error mean absolute error mean absolute percent error standard deviation median median absolute deviation interquartile range linear ﬁt slope linear ﬁt intercept Kendall τ correlation

0 0 0 0 0 0 0 1 0 1

HSE

B3PW91

B3LYP

PBE0

27

41

27

37

27

34

27

−0.24 0.37 16 0.55 −0.06 0.21 0.49 0.79 0.36 0.85

−0.21 0.38 15 0.54 −0.07 0.27 0.50 0.87 0.23 0.88

0.14 0.44 27 0.53 0.33 0.25 0.57 0.82 0.65 0.85

0.12 0.41 26 0.51 0.29 0.29 0.55 0.82 0.65 0.88

0.13 0.44 23 0.56 0.19 0.34 0.69 0.82 0.63 0.84

0.16 0.47 25 0.56 0.27 0.3 0.73 0.81 0.70 0.85

0.43 0.59 45 0.50 0.63 0.14 0.43 0.82 0.95 0.86

4166

DOI: 10.1021/acs.jpclett.6b01807 J. Phys. Chem. Lett. 2016, 7, 4165−4170

Letter

The Journal of Physical Chemistry Letters

Table 2. Wilcoxon Signed-Rank Test W Values for the Absolute Errors of Pairs of Hybrid Functionals Using the Data That Appears in Figure 1 along with Associated p Values in Parenthesesa

The following three statistics of the deviations from experiment in Table 1, the median, the median absolute deviation, and the interquartile range, are measures taken from robust statistics, which are more resilient to outliers as compared to the ME, MAE, and SD. In statistics, the median is considered a better descriptor of typical outcome than the mean when the latter is biased by outliers; the median absolute deviation measures statistical dispersion (in this case of the error), and the interquartile range measures the variability in a set of data. For a method that perfectly predicts band gaps, all of these values must be zero. We observe, as before, that diﬀerent functionals provide the best results for diﬀerent error measures; HSE has the best median and PBE0 the worst, but the latter has the best median absolute deviation and interquartile range. Note, however, that the median absolute deviation and the interquartile range of HSE are only 0.06 eV larger than those of PBE0, while the median of HSE is 0.53 eV closer to zero than the median of PBE0. Thus, overall, measures from robust statistics favor HSE the most. Apart from the various statistics analyzed so far, an important feature of a quantum chemical method is its ability to correctly reproduce trends. A trend can be deﬁned by a linear ﬁt as follows yexpt = mycalc + b

HSE B3PW91 B3LYP PBE0

B3LYP

PBE0

42(0.61) − 18(0.83) 227(0.01)

84(0.31) 18(0.83) − 214(0.01)

128(0.14) 227(0.01) 214(0.01) −

The value for Wcrit with a 95% conﬁdence interval is 107; W < Wcrit for a pair of methods indicates that their absolute errors show the same statistical distribution at around zero.

methods) follows a symmetric distribution around zero because each set has the same statistical distribution, resulting in similar positive and negative diﬀerences; the null hypothesis is rejected when the test statistic W is greater than a certain Wcrit determined by the sample size and level of conﬁdence. A p value associated with the test represents the probability of obtaining the observed distribution, or a more asymmetric distribution around zero, assuming that the null hypothesis is true; p values larger than 0.05 have been related to a lack of meaningful diﬀerence in the context of method comparison.15 On the basis of both the W test statistic and its associated p values, the results in Table 2 indicate no signiﬁcant statistical diﬀerence (considering a commonly used 95% conﬁdence interval) in the absolute error distributions of HSE, B3PW91, and B3LYP. The W statistics suggest, however, that diﬀerences exist between these three functionals and PBE0; the p values also imply a signiﬁcant diﬀerence between PBE0 and both B3PW91 and B3LYP. If the same analysis is carried out for the signed error and absolute percentage error, all pairs of functionals come out as being statistically diﬀerent except for the B3PW91/B3LYP pair. The results of the Wilcoxon signedrank test support the more qualitative comparison of the ME, MAE, and MAPE discussed above and put such a discussion in a rigorous statistical framework. On the Underestimation of Large Band Gaps. As shown here and in other works,10 even hybrid functionals underestimate band gaps when these are considerably large. No single hybrid with a ﬁxed amount of HF exchange can accurately describe small and large band gap materials simultaneously; the fraction of nonlocal exchange needed in a solid depends on its dielectric function.15−17 Increasing the percentage of HF exchange in a hybrid functional increases the band gap, which allows for the description of larger band gap insulators but causes overestimation of semiconductor band gaps. A way to optimize the fraction of HF exchange in hybrid functionals based on a local estimator of the dielectric function has been proposed in ref 16. With this procedure, one ﬁnds, for example, that HSE predicts a band gap 22.29 eV for solid Ne (which has an experimental gap of 21.70 eV) while still giving good semiconductor band gaps (e.g., 0.82 eV for Ge, compared to 0.74 eV from experiment).16 The method is applicable to global hybrids too; an optimized PBE0 gives gaps of 21.88 and 0.68 eV for Ne and Ge, respectively, compared to 15.14 and 1.31 eV predicted by standard PBE0.16 As another example of how even screened hybrids can describe large band gap insulators, consider the HSE-HF functional of ref 18, which is simply HSE06 but with 100% exact exchange in the short-range. Figure 2 shows the band gap of NaCl calculated by HSE-HF as a function of the range

(1)

P−Q (P + Q + T )(P + Q + U )

B3PW91

− 42(0.61) 84(0.31) 128(0.14)

a

Table 1 shows the values of the slope m and the intercept b from this linear ﬁt for the band gaps calculated by the four hybrid functionals. Ideally, m = 1 and b = 0. Judging by the values of the slopes, the four hybrids have a similar quality for predicting trends; the slopes are all around 0.80 and do not diﬀer by more than about 3%. However, PBE0 has a substantially higher intercept (0.95 eV) than other methods, whereas HSE is closest to zero (0.36 eV), and B3PW91 and B3LYP are in between that (∼0.65 eV). Hence, with respect to trends, all functionals are similar, but HSE appears to be slightly better again. Last, let us consider a measure of rank correlation to judge the quality of predicted band gaps: the Kendall τ rank correlation coeﬃcient. In order to construct this coeﬃcient, calc expt we ﬁrst need to deﬁne the pairs (gexpt and gcalc i , gi ), where gi i are the experimental and calculated gaps, respectively. The pairs i and j are then said to be concordant if gexpt < gexpt and gcalc < i j i expt expt calc calc gcalc or if g > g and g > g , tied if g = g , and discordant j i j i j i j otherwise. The Kendall τ correlation coeﬃcient is then τ=

HSE

(2)

where P is the number of concordant pairs, Q the number of discordant pairs, and T and U the number of ties in the experimental and calculated set of band gaps, respectively. Thus, τ measures the similarity in the orderings of two data sets; a τ value of 1 indicates perfect agreement in the ordering, whereas τ = −1 indicates complete disagreement. It can, in a way, be considered a measure of qualitative agreement. We see in Table 1 that all four hybrids provide essentially the same τ value (∼0.85) and thus have all similarly good qualitative agreement with experiment. One could also analyze the distribution of the error of pairs of methods and ask whether the distributions diﬀer statistically. This is done in Table 2 using the Wilcoxon signed-rank test for the absolute error data. The null hypothesis of the test is that the diﬀerence between pairs (of absolute errors for two 4167

DOI: 10.1021/acs.jpclett.6b01807 J. Phys. Chem. Lett. 2016, 7, 4165−4170

Letter

The Journal of Physical Chemistry Letters

3.06 eV).9 However, this approach may not be appropriate in this case; the experimentally reported 5.43 eV value is most likely the direct gap, whereas the smaller values correspond to the indirect gap.21 Even if one decided to follow this methodology, the SD of the six experimental band gap values for CoO is 1.22 eV, and hence, all functionals predicting values in the wide range between 1.90 and 4.34 eV would have to be considered to be in agreement with experiment. The often cited value of 2.5 eV for the CoO band gap is in reasonable agreement with the HSE indirect gap of 2.82 eV. An additional consequence of the variability in the reference data is that small diﬀerences in the average errors of diﬀerent functionals are not really meaningful. Thus, on the basis of, say, the MAEs in Table 1, it would be hard to tell whether HSE, B3PW91, or B3LYP is truly closer to experiment. Furthermore, adding to the level of uncertainty, experimental reference band gaps are assumed to be an ideal measurement of the fundamental band gap (i.e., the diﬀerence between the ionization potential and electron aﬃnity). However, this is not always the case,10 whereas the calculation of generalized Kohn−Sham band gaps (as done here) is a rigorous and honest approximation to the fundamental band gap.22 Considering all of this and the fact that the use of diﬀerent, ﬁnite basis sets leads to further changes in predicted band gaps, it would be unreasonable to assert that a certain functional is decidedly better than another for band gap predictions if the diﬀerences in the error measures are small (e.g., less than about 0.1 eV or, depending on the case, even more than this, as shown by the CoO example above). Statistical methods such as the ones used here should be considered for assessing whether the diﬀerences are signiﬁcant. The importance of careful inspection of reference data from the literature and the use of a consistent methodology in benchmark calculations applies to not only density functionals. The GW method, for example, is quite sensitive to a number of variables: the input (reference) wave function, number of empty bands included, dielectric matrix energy cutoﬀ, and so forth. To illustrate this, consider the GW band gaps of ZnO used as reference to compare against B3PW91 in the Supporting Information of ref 9. The experimental band gap is 3.44 eV; the GW gaps in the literature vary from 0.1 to 4.61 eV. The worst value, 0.1 eV, was computed using the static Coulomb hole and screened exchange (COHSEX) approximation, which is generally not recommended for quantitative calculations.23 Shih et al.24 report that conventional GW approaches can provide accurate estimates of the ZnO band gap if convergence in the evaluation of the Coulomb-hole selfenergy is carefully resolved. Further examples with large variability (more than 1 eV) in the GW gaps cited in ref 9 include Si (0.56−1.91), GaAs (1.09−3.77), SiC (1.8−2.88), AlP (1.88−3.1), CdS (2.11−3.41), CoO (2.4−4.78), GaN (2.75−3.82), MnO (2.34−4.39), ZnS (1.52−4.15), NiO (1.74−5.0), diamond (5.59−6.99), LiCl (8.75−10.98), and LiF (13.13−16.17) among others. It is worth pointing out here that ref 9 concluded that B3PW91 was superior to other functionals by comparing against GW, assuming that GW is more accurate than these (other) functionals. However, as shown here, such comparisons are not straightforward, and B3PW91 does not appear to have any decisive advantage over other commonly used hybrids when the direct comparison is done using identical geometries, basis sets, and so forth. The eﬀects of spin−orbit coupling should also be mentioned here. We have not included these eﬀects in our calculations as such corrections are not widely available in commercial codes.

Figure 2. NaCl band gap calculated by HSE-HF (HSE06 wtih 100% exact exchange) as a function of the range separation parameter.

separation parameter, ω. The smaller this parameter, the larger the fraction of HF exchange incorporated. At small ω values, the band gap is overestimated; at ω ≈ 0.2−0.3 au, the value is close to experiment, and at higher ω values, the gap is underestimated. This is just one example, but this behavior is very general, and this observation is in agreement with previous works showing that long-range HF exchange is seldom necessary and that the physics behind the more realistic properties computed with hybrid functionals is the reduction of the self-interaction error by incorporation of substantial amounts of exact exchange.18,19 Thus, a short-range screened hybrid can describe even large band gap insulators, and one does not need to resort to more expensive global hybrids. Note also that although, in principle, long-range HF exchange should be included when describing solids, its eﬀect should be mostly canceled by correlation. Inadequate treatment of correlation is the reason why the HF method and typical global hybrid functionals cannot describe metallic behavior. Hence, it is convenient to eliminate long-range exchange and use a screened hybrid to more adequately describe the physics of an extended solid. Additional Considerations. We have focused on band gaps calculated using experimental geometries and observed little overall diﬀerence between the diﬀerent hybrids tested. However, other properties, including geometries, can be signiﬁcantly diﬀerent. For example, the MAE of B3LYP for lattice constants (0.053 Å) is more than twice larger than the MAEs of HSE and PBE0 (0.024 and 0.022 Å, respectively).20 Atomization energies of solids are also signiﬁcantly worse when calculated with B3LYP (MAE = 0.59 eV) as compared to HSE and PBE0 (MAE ≈ 0.26 eV); B3PW91 improves over B3LYP, but it is not as good as the latter two functionals (MAE = 0.39 eV).20 The failure of B3LYP is attributed to not correctly reproducing the homogeneous electron gas behavior, and B3PW91 improves upon it by fulﬁlling this limit.20 Even when considering only band gaps and using experimental geometries, another important consideration arises: the quality of the experimental data. In particular for the band gaps, there can be a signiﬁcant variability depending on factors such as the method of measurement and temperature (which sometimes is not reported). For example, band gap values of 3.6, 2.6, 2.5, 2.1, 2.7, and 5.43 eV have been reported for CoO (see the Supporting Information of ref 9). This variability leads to the question: What value should one use as reference? One can average all of these values (3.16 eV) and obtain very good agreement with B3PW91 (calculated here as 4168

DOI: 10.1021/acs.jpclett.6b01807 J. Phys. Chem. Lett. 2016, 7, 4165−4170

The Journal of Physical Chemistry Letters

■

Nevertheless, our conclusions are not aﬀected by neglecting spin−orbit coupling because of, mainly, two reasons. The ﬁrst one is that we have not included compounds for which spin− orbit coupling eﬀects are important in our test set. The second one is related to the fact that spin−orbit corrections apply in the same way to all functionals; that is, if we use experimental spin−orbit coupling values to correct the band gaps, the shift in the error is the same for every functional. Here, we observe that various hybrids provide rather similar results, with no clear winner in all cases and a diﬀerent method being “better” depending on the error measure. After spin−orbit coupling corrections, the functionals will still provide similar results because these corrections are identical for all of them. Last, an important consideration for calculations on extended systems is computational cost. The increase in CPU time when going from a semilocal functional, to a screened hybrid, to a global hybrid depends on the type of basis set employed. Here, we have used codes based on localized Gaussian basis sets, which are not as eﬃcient for semilocal functionals but have a less dramatic increase in cost for hybrids as compared to planewave-based codes. This means that in plane-wave implementations of DFT screened hybrids are more strongly favored over global hybrids concerning CPU time. After carrying out a thorough comparison between four popular hybrid functionals for predicting band gaps using a consistent methodology in the calculations, we did not ﬁnd truly signiﬁcant diﬀerences in the overall performance of three of them: HSE, B3PW91, and B3LYP (the latter two in particular give very similar gaps). PBE0 tends to overestimate band gaps, but the error is systematic and the statistical analysis shows that all four functionals provide good qualitative agreement with the reference data. Nevertheless, our results do suggest that HSE is more accurate for typical semiconductors. The analysis here shows that there is nothing particularly remarkable about the band gaps predicted by B3PW919 when they are compared to other global hybrids using a similar amount of HF exchange. We have also shown how screened hybrids can incorporate larger fractions of HF exchange in the short-range to compensate for the eﬀects that result from screening in large gap insulators, and ways to tune the mixing parameter that solve this problem have also been proposed in the literature.15−17 Global hybrids also underestimate very large band gaps and can too be modiﬁed to include more exchange to solve this problem, but at a higher computational cost. Thus, on the basis of cost and accuracy considerations, we recommend HSE for semiconductors and tuned versions of HSE for larger gap cases. In summary, screened hybrids can describe the same type of problems that global hybrids do, but in addition, they provide access to modeling metallic behavior, have a much lower computational cost, and are easier to converge. Our conclusion is therefore that a screened hybrid like HSE is preferable over global hybrids for the black box prediction of band gaps of novel materials.

■

Letter

AUTHOR INFORMATION

Corresponding Author

*E-mail: [email protected] Present Address ¶

A.J.G.: The Joint Center for Artiﬁcial Photosynthesis, Lawrence Berkeley National Laboratory, Berkeley, California 94720, USA.

Notes

The authors declare no competing ﬁnancial interest.

■

ACKNOWLEDGMENTS This work was supported as part of the Center for the Computational Design of Functional Layered Materials, an Energy Frontier Research Center funded by the U.S. Department of Energy, Oﬃce of Science, Basic Energy Sciences under Award [# DE-SC0012575]. G.E.S. is a Welch Foundation chair (C-0036). We also thank the authors of ref 15 for bringing their paper to our attention and suggesting the use of the Wilcoxon signed-rank test.

■

REFERENCES

(1) Perdew, J. P.; Levy, M. Physical Content of the Exact Kohn− Sham Orbital Energies: Band Gaps and Derivative Discontinuities. Phys. Rev. Lett. 1983, 51, 1884−1887. (2) Mori-Sánchez, P.; Cohen, A. J.; Yang, W. Localization and Delocalization Errors in Density Functional Theory and Implications for Band-Gap Prediction. Phys. Rev. Lett. 2008, 100, 146401. (3) Heyd, J.; Scuseria, G. E.; Ernzerhof, M. Hybrid Functionals Based on a Screened Coulomb Potential. J. Chem. Phys. 2003, 118, 8207− 8215. (4) Heyd, J.; Scuseria, G. E.; Ernzerhof, M. Erratum: “Hybrid functionals based on a screened Coulomb potential. J. Chem. Phys. 2006, 124, 219906. (5) Henderson, T. M.; Izmaylov, A. F.; Scuseria, G. E.; Savin, A. The Importance of Middle-Range Hartree-Fock-type Exchange for Hybrid Density Functionals. J. Chem. Phys. 2007, 127, 221103. (6) Moussa, J. E.; Schultz, P. A.; Chelikowsky, J. R. Analysis of the Heyd-Scuseria-Ernzerhof Density Functional Parameter Space. J. Chem. Phys. 2012, 136, 204117. (7) Lucero, M. J.; Henderson, T. M.; Scuseria, G. E. Improved Semiconductor Lattice Parameters and Band Gaps from a MiddleRange Screened Hybrid Exchange functional. J. Phys.: Condens. Matter 2012, 24, 145504. (8) Henderson, T. M.; Paier, J.; Scuseria, G. E. Accurate treatment of solids with the HSE Screened Hybrid. Phys. Status Solidi B 2011, 248, 767−774. (9) Crowley, J. M.; Tahir-Kheli, J.; Goddard, W. A., III Resolution of the Band Gap Prediction Problem for Materials Design. J. Phys. Chem. Lett. 2016, 7, 1198−1203. (10) Civalleri, B.; Presti, D.; Dovesi, R.; Savin, A. On Choosing the Best Density Functional Approximation. Chem. Modell. 2012, 9, 168− 185. (11) Savin, A.; Johnson, E. Judging Density-Functional Approximations: Some Pitfalls of Statistics. Top. Curr. Chem. 2014, 365, 81− 96. (12) Heyd, J. Screened Coulomb Hybrid Density Functionals. Ph.D. Dissertation, Rice University, Houston, TX, 2004. (13) Frisch, M. J.; Trucks, G. W.; Schlegel, H. B.; Scuseria, G. E.; Robb, M. A.; Cheeseman, J. R.; Scalmani, G.; Barone, V.; Mennucci, B.; Petersson, G. A. et al. Gaussian 09, revision A.02; Gaussian Inc.: Wallingford, CT, 2009. (14) Natiello, M. A.; Scuseria, G. E. Convergence properties of Hartree-Fock SCF Molecular Calculations. Int. J. Quantum Chem. 1984, 26, 1039.

ASSOCIATED CONTENT

S Supporting Information *

The Supporting Information is available free of charge on the ACS Publications website at DOI: 10.1021/acs.jpclett.6b01807. Details about the calculations, as well as band gap data used in this work (PDF) 4169

DOI: 10.1021/acs.jpclett.6b01807 J. Phys. Chem. Lett. 2016, 7, 4165−4170

Letter

The Journal of Physical Chemistry Letters (15) Skone, J. H.; Govoni, M.; Galli, G. Nonempirical RangeSeparated Hybrid Functionals for Solids and Molecules. Phys. Rev. B 2016, 93, 235106. (16) Marques, M. A. L.; Vidal, J.; Oliveira, M. J. T.; Reining, L.; Botti, S. Density-based Mixing Parameter for Hybrid Functionals. Phys. Rev. B 2011, 83, 035119. (17) Skone, J. H.; Govoni, M.; Galli, G. Self-Consistent Hybrid Functional for Condensed Systems. Phys. Rev. B 2014, 89, 195112. (18) Garza, A. J.; Wazzan, N. A.; Asiri, A. M.; Scuseria, G. E. Can Short- and Middle-Range Hybrids Describe the Hyperpolarizabilities of Long-Range Charge-Transfer Compounds? J. Phys. Chem. A 2014, 118, 11787−11796. (19) Henderson, T. M.; Izmaylov, A. F.; Scalmani, G.; Scuseria, G. E. Can Short-Range Hybrids Describe Long-Range-Dependent Properties? J. Chem. Phys. 2009, 131, 044108. (20) Paier, J.; Marsman, M.; Kresse, G. Why Does the B3LYP Hybrid Functional Fail for Metals? J. Chem. Phys. 2007, 127, 024103. (21) Gillen, R.; Robertson, J. Accurate Screened Exchange Band Structures for the Transition Metal Monoxides MnO, FeO, CoO and NiO. J. Phys.: Condens. Matter 2013, 25, 165502. (22) Perdew, J. P.; Yang, W.; Burke, K.; Yang, Z.; Gross, E. K. U.; Scheﬄer, M.; Scuseria, G. E.; Henderson, T. M.; Zhang, I. Y.; Ruzsinszky, A.; Peng, H.; Sun, J. Understanding Band Gaps of Solids in Generalized Kohn-Sham Theory. arXiv:1608.06715. arXiv.org ePrint archive. https://arxiv.org/abs/1608.06715 (accessed Oct 2, 2016). (23) Hüser, F.; Olsen, T.; Thygesen, K. S. Quasiparticle GW Calculations for Solids, Molecules, and Two-Dimensional Materials. Phys. Rev. B 2013, 87, 235132. (24) Shih, B.-C.; Xue, Y.; Zhang, P.; Cohen, M. L.; Louie, S. G. Quasiparticle Band Gap of ZnO: High Accuracy from the Conventional G0W0 Approach. Phys. Rev. Lett. 2010, 105, 146401.

4170

DOI: 10.1021/acs.jpclett.6b01807 J. Phys. Chem. Lett. 2016, 7, 4165−4170